# Electronic Supplementary Material (ESI) for Chemical Science.
# This journal is © The Royal Society of Chemistry 2022

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_2
_database_code_depnum_ccdc_archive 'CCDC 2164005'
loop_
_audit_author_name
_audit_author_address
'Yilei Hu'
;Tongji University
China
;
_audit_update_record             
;
2022-04-02 deposited with the CCDC.	2022-07-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'Cs2 F5 I O4 W'
_chemical_formula_weight         735.57

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Cs Cs -0.3680 2.1192 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           36
_space_group_name_H-M_alt        'C m c 21'
_space_group_name_Hall           'C 2c -2'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, z'
'x, -y, z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z+1/2'

_cell_length_a                   12.1122(6)
_cell_length_b                   10.6192(6)
_cell_length_c                   7.8333(4)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     1007.53(9)
_cell_formula_units_Z            4
_cell_measurement_temperature    294(2)
_cell_measurement_reflns_used    2424
_cell_measurement_theta_min      3.6438
_cell_measurement_theta_max      27.0656

_exptl_crystal_description       rob-like
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.849
_exptl_crystal_F_000             1256
_exptl_transmission_factor_min   ?
_exptl_transmission_factor_max   ?
_exptl_crystal_size_max          ?
_exptl_crystal_size_mid          ?
_exptl_crystal_size_min          ?
_exptl_absorpt_coefficient_mu    21.707
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      294(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  "SADABS; Bruker, 2000''SADABS; Bruker, 2000"
_diffrn_measurement_method       ?
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            2933
_diffrn_reflns_av_unetI/netI     0.0498
_diffrn_reflns_av_R_equivalents  0.0342
_diffrn_reflns_limit_h_min       -15
_diffrn_reflns_limit_h_max       15
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_k_max       10
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_limit_l_max       10
_diffrn_reflns_theta_min         2.551
_diffrn_reflns_theta_max         27.083
_diffrn_reflns_theta_full        25.242
_diffrn_measured_fraction_theta_max 0.998
_diffrn_measured_fraction_theta_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.998
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.999
_diffrn_reflns_point_group_measured_fraction_full 0.999
_reflns_number_total             1111
_reflns_number_gt                1085
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.858
_reflns_Friedel_fraction_max     1.000
_reflns_Friedel_fraction_full    1.000

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0172P)²] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     'SHELXL-2017/1 (Sheldrick 2017)'
_refine_ls_extinction_coef       0.0046(2)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.02(2)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         1111
_refine_ls_number_parameters     45
_refine_ls_number_restraints     1
_refine_ls_R_factor_all          0.0291
_refine_ls_R_factor_gt           0.0279
_refine_ls_wR_factor_ref         0.0604
_refine_ls_wR_factor_gt          0.0599
_refine_ls_goodness_of_fit_ref   1.083
_refine_ls_restrained_S_all      1.083
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.500000 1.18078(7) 0.64347(10) 0.0201(2) Uani 1 2 d S T P . .
I1 I 0.500000 1.46738(11) 0.93986(14) 0.0173(3) Uani 1 2 d S T P . .
O1 O 0.500000 1.3526(14) 1.1018(18) 0.027(3) Uiso 1 2 d S . P . .
F1 F 0.6630(7) 1.4638(10) 0.9390(12) 0.041(2) Uiso 1 1 d . . . . .
O2 O 0.500000 1.3806(16) 0.744(2) 0.037(4) Uiso 1 2 d S . P . .
F2 F 0.6046(6) 1.2641(9) 0.4910(10) 0.0291(18) Uiso 1 1 d . . . . .
O3 O 0.6126(8) 1.1543(10) 0.7891(12) 0.024(2) Uiso 1 1 d . . . . .
F3 F 0.500000 1.0363(15) 0.5406(19) 0.050(4) Uiso 1 2 d S . P . .
Cs1 Cs 0.81374(6) 1.35275(9) 0.66501(11) 0.0287(3) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 F3 1.733(16) . ?
W1 O3 1.800(10) 3_655 ?
W1 O3 1.800(10) . ?
W1 F2 1.953(8) 3_655 ?
W1 F2 1.953(8) . ?
W1 O2 2.263(17) . ?
W1 Cs1 4.1536(12) 5_445 ?
W1 Cs1 4.1536(12) 7_645 ?
W1 Cs1 4.2195(9) . ?
W1 Cs1 4.2195(9) 3_655 ?
W1 Cs1 4.3889(11) 8_474 ?
W1 Cs1 4.3889(11) 6_674 ?
I1 O1 1.759(14) . ?
I1 O2 1.790(17) . ?
I1 F1 1.974(8) 3_655 ?
I1 F1 1.974(8) . ?
I1 Cs1 4.4448(14) 8_475 ?
I1 Cs1 4.4448(14) 6_675 ?
O1 Cs1 3.176(10) 8_475 ?
O1 Cs1 3.176(10) 6_675 ?
F1 Cs1 3.055(9) . ?
F1 Cs1 3.203(9) 4_585 ?
F2 Cs1 3.006(8) 6_674 ?
F2 Cs1 3.026(8) . ?
O3 Cs1 3.077(10) 6_675 ?
O3 Cs1 3.365(10) . ?
O3 Cs1 3.463(10) 7_645 ?
F3 Cs1 3.137(11) 5_445 ?
F3 Cs1 3.137(11) 7_645 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F3 W1 O3 99.0(5) . 3_655 ?
F3 W1 O3 99.0(5) . . ?
O3 W1 O3 98.5(6) 3_655 . ?
F3 W1 F2 96.7(5) . 3_655 ?
O3 W1 F2 88.1(4) 3_655 3_655 ?
O3 W1 F2 161.8(4) . 3_655 ?
F3 W1 F2 96.7(5) . . ?
O3 W1 F2 161.8(4) 3_655 . ?
O3 W1 F2 88.1(4) . . ?
F2 W1 F2 80.9(5) 3_655 . ?
F3 W1 O2 172.6(7) . . ?
O3 W1 O2 85.8(4) 3_655 . ?
O3 W1 O2 85.8(4) . . ?
F2 W1 O2 77.8(4) 3_655 . ?
F2 W1 O2 77.8(4) . . ?
F3 W1 Cs1 43.7(3) . 5_445 ?
O3 W1 Cs1 55.4(3) 3_655 5_445 ?
O3 W1 Cs1 104.7(3) . 5_445 ?
F2 W1 Cs1 93.0(3) 3_655 5_445 ?
F2 W1 Cs1 139.2(3) . 5_445 ?
O2 W1 Cs1 140.6(2) . 5_445 ?
F3 W1 Cs1 43.7(3) . 7_645 ?
O3 W1 Cs1 104.8(3) 3_655 7_645 ?
O3 W1 Cs1 55.4(3) . 7_645 ?
F2 W1 Cs1 139.2(3) 3_655 7_645 ?
F2 W1 Cs1 93.0(3) . 7_645 ?
O2 W1 Cs1 140.6(2) . 7_645 ?
Cs1 W1 Cs1 65.80(3) 5_445 7_645 ?
F3 W1 Cs1 113.69(10) . . ?
O3 W1 Cs1 136.4(3) 3_655 . ?
O3 W1 Cs1 50.2(3) . . ?
F2 W1 Cs1 114.4(3) 3_655 . ?
F2 W1 Cs1 40.9(2) . . ?
O2 W1 Cs1 65.18(6) . . ?
Cs1 W1 Cs1 148.27(3) 5_445 . ?
Cs1 W1 Cs1 82.657(9) 7_645 . ?
F3 W1 Cs1 113.69(10) . 3_655 ?
O3 W1 Cs1 50.2(3) 3_655 3_655 ?
O3 W1 Cs1 136.4(3) . 3_655 ?
F2 W1 Cs1 40.9(2) 3_655 3_655 ?
F2 W1 Cs1 114.4(3) . 3_655 ?
O2 W1 Cs1 65.18(6) . 3_655 ?
Cs1 W1 Cs1 82.656(9) 5_445 3_655 ?
Cs1 W1 Cs1 148.27(3) 7_645 3_655 ?
Cs1 W1 Cs1 128.48(3) . 3_655 ?
F3 W1 Cs1 62.0(4) . 8_474 ?
O3 W1 Cs1 98.0(3) 3_655 8_474 ?
O3 W1 Cs1 156.6(3) . 8_474 ?
F2 W1 Cs1 35.0(3) 3_655 8_474 ?
F2 W1 Cs1 81.3(2) . 8_474 ?
O2 W1 Cs1 111.9(4) . 8_474 ?
Cs1 W1 Cs1 71.790(19) 5_445 8_474 ?
Cs1 W1 Cs1 104.23(2) 7_645 8_474 ?
Cs1 W1 Cs1 122.15(3) . 8_474 ?
Cs1 W1 Cs1 66.817(16) 3_655 8_474 ?
F3 W1 Cs1 62.0(4) . 6_674 ?
O3 W1 Cs1 156.6(3) 3_655 6_674 ?
O3 W1 Cs1 98.0(3) . 6_674 ?
F2 W1 Cs1 81.3(2) 3_655 6_674 ?
F2 W1 Cs1 35.0(3) . 6_674 ?
O2 W1 Cs1 111.9(4) . 6_674 ?
Cs1 W1 Cs1 104.23(2) 5_445 6_674 ?
Cs1 W1 Cs1 71.790(19) 7_645 6_674 ?
Cs1 W1 Cs1 66.817(16) . 6_674 ?
Cs1 W1 Cs1 122.15(3) 3_655 6_674 ?
Cs1 W1 Cs1 61.86(2) 8_474 6_674 ?
O1 I1 O2 105.2(7) . . ?
O1 I1 F1 89.4(3) . 3_655 ?
O2 I1 F1 89.3(3) . 3_655 ?
O1 I1 F1 89.4(3) . . ?
O2 I1 F1 89.3(3) . . ?
F1 I1 F1 177.8(6) 3_655 . ?
O1 I1 Cs1 35.3(2) . 8_475 ?
O2 I1 Cs1 86.9(5) . 8_475 ?
F1 I1 Cs1 58.6(3) 3_655 8_475 ?
F1 I1 Cs1 119.6(3) . 8_475 ?
O1 I1 Cs1 35.3(2) . 6_675 ?
O2 I1 Cs1 86.9(5) . 6_675 ?
F1 I1 Cs1 119.6(3) 3_655 6_675 ?
F1 I1 Cs1 58.6(3) . 6_675 ?
Cs1 I1 Cs1 61.00(3) 8_475 6_675 ?
I1 O1 Cs1 126.0(4) . 8_475 ?
I1 O1 Cs1 126.0(4) . 6_675 ?
Cs1 O1 Cs1 90.5(4) 8_475 6_675 ?
I1 F1 Cs1 127.4(4) . . ?
I1 F1 Cs1 123.8(4) . 4_585 ?
Cs1 F1 Cs1 106.4(2) . 4_585 ?
I1 O2 W1 141.3(9) . . ?
W1 F2 Cs1 123.1(4) . 6_674 ?
W1 F2 Cs1 114.1(3) . . ?
Cs1 F2 Cs1 103.6(2) 6_674 . ?
W1 O3 Cs1 146.1(5) . 6_675 ?
W1 O3 Cs1 105.5(4) . . ?
Cs1 O3 Cs1 94.7(3) 6_675 . ?
W1 O3 Cs1 99.3(4) . 7_645 ?
Cs1 O3 Cs1 99.9(3) 6_675 7_645 ?
Cs1 O3 Cs1 108.2(3) . 7_645 ?
W1 F3 Cs1 113.9(4) . 5_445 ?
W1 F3 Cs1 113.9(4) . 7_645 ?
Cs1 F3 Cs1 92.0(4) 5_445 7_645 ?
F2 Cs1 F2 121.97(15) 6_675 . ?
F2 Cs1 F1 76.1(2) 6_675 . ?
F2 Cs1 F1 86.3(2) . . ?
F2 Cs1 O3 135.0(2) 6_675 6_674 ?
F2 Cs1 O3 78.7(2) . 6_674 ?
F1 Cs1 O3 148.7(3) . 6_674 ?
F2 Cs1 F3 106.5(3) 6_675 5 ?
F2 Cs1 F3 130.9(3) . 5 ?
F1 Cs1 F3 114.1(3) . 5 ?
O3 Cs1 F3 60.6(3) 6_674 5 ?
F2 Cs1 O1 67.4(3) 6_675 6_674 ?
F2 Cs1 O1 108.1(3) . 6_674 ?
F1 Cs1 O1 143.1(3) . 6_674 ?
O3 Cs1 O1 68.2(3) 6_674 6_674 ?
F3 Cs1 O1 82.4(3) 5 6_674 ?
F2 Cs1 F1 155.2(2) 6_675 4_584 ?
F2 Cs1 F1 57.5(2) . 4_584 ?
F1 Cs1 F1 79.20(15) . 4_584 ?
O3 Cs1 F1 69.6(3) 6_674 4_584 ?
F3 Cs1 F1 82.0(3) 5 4_584 ?
O1 Cs1 F1 137.4(3) 6_674 4_584 ?
F2 Cs1 O3 74.6(2) 6_675 . ?
F2 Cs1 O3 47.9(2) . . ?
F1 Cs1 O3 66.8(3) . . ?
O3 Cs1 O3 118.1(2) 6_674 . ?
F3 Cs1 O3 178.7(3) 5 . ?
O1 Cs1 O3 97.4(3) 6_674 . ?
F1 Cs1 O3 97.3(2) 4_584 . ?
F2 Cs1 O3 93.4(2) 6_675 7_655 ?
F2 Cs1 O3 129.0(2) . 7_655 ?
F1 Cs1 O3 66.4(2) . 7_655 ?
O3 Cs1 O3 102.5(2) 6_674 7_655 ?
F3 Cs1 O3 47.7(3) 5 7_655 ?
O1 Cs1 O3 119.7(2) 6_674 7_655 ?
F1 Cs1 O3 74.9(2) 4_584 7_655 ?
O3 Cs1 O3 133.2(3) . 7_655 ?
F2 Cs1 W1 101.66(17) 6_675 5 ?
F2 Cs1 W1 134.19(17) . 5 ?
F1 Cs1 W1 91.68(19) . 5 ?
O3 Cs1 W1 79.86(19) 6_674 5 ?
F3 Cs1 W1 22.4(3) 5 5 ?
O1 Cs1 W1 100.58(19) 6_674 5 ?
F1 Cs1 W1 77.13(16) 4_584 5 ?
O3 Cs1 W1 158.48(17) . 5 ?
O3 Cs1 W1 25.32(16) 7_655 5 ?
F2 Cs1 W1 98.72(16) 6_675 . ?
F2 Cs1 W1 25.00(15) . . ?
F1 Cs1 W1 69.93(17) . . ?
O3 Cs1 W1 102.26(18) 6_674 . ?
F3 Cs1 W1 154.7(2) 5 . ?
O1 Cs1 W1 109.65(19) 6_674 . ?
F1 Cs1 W1 74.19(16) 4_584 . ?
O3 Cs1 W1 24.28(17) . . ?
O3 Cs1 W1 130.04(16) 7_655 . ?
W1 Cs1 W1 148.27(3) 5 . ?
F2 Cs1 W1 21.90(17) 6_675 6_675 ?
F2 Cs1 W1 142.15(16) . 6_675 ?
F1 Cs1 W1 74.85(17) . 6_675 ?
O3 Cs1 W1 131.76(18) 6_674 6_675 ?
F3 Cs1 W1 86.9(2) 5 6_675 ?
O1 Cs1 W1 73.3(2) 6_674 6_675 ?
F1 Cs1 W1 144.51(17) 4_584 6_675 ?
O3 Cs1 W1 94.28(17) . 6_675 ?
O3 Cs1 W1 72.71(16) 7_655 6_675 ?
W1 Cs1 W1 79.84(2) 5 6_675 ?
W1 Cs1 W1 117.51(2) . 6_675 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O2 I1 O1 Cs1 -61.4(6) . . . 8_475 ?
F1 I1 O1 Cs1 27.7(7) 3_655 . . 8_475 ?
F1 I1 O1 Cs1 -150.5(7) . . . 8_475 ?
Cs1 I1 O1 Cs1 -122.9(12) 6_675 . . 8_475 ?
O2 I1 O1 Cs1 61.4(6) . . . 6_675 ?
F1 I1 O1 Cs1 150.5(7) 3_655 . . 6_675 ?
F1 I1 O1 Cs1 -27.7(7) . . . 6_675 ?
Cs1 I1 O1 Cs1 122.9(12) 8_475 . . 6_675 ?
O1 I1 O2 W1 0.000(10) . . . . ?
F1 I1 O2 W1 -89.2(3) 3_655 . . . ?
F1 I1 O2 W1 89.2(3) . . . . ?
Cs1 I1 O2 W1 -30.55(3) 8_475 . . . ?
Cs1 I1 O2 W1 30.55(3) 6_675 . . . ?
F3 W1 O3 Cs1 -122.2(9) . . . 6_675 ?
O3 W1 O3 Cs1 -21.6(12) 3_655 . . 6_675 ?
F2 W1 O3 Cs1 88.7(15) 3_655 . . 6_675 ?
F2 W1 O3 Cs1 141.3(9) . . . 6_675 ?
O2 W1 O3 Cs1 63.5(9) . . . 6_675 ?
Cs1 W1 O3 Cs1 -77.9(9) 5_445 . . 6_675 ?
Cs1 W1 O3 Cs1 -123.7(10) 7_645 . . 6_675 ?
Cs1 W1 O3 Cs1 124.4(10) . . . 6_675 ?
Cs1 W1 O3 Cs1 17.0(12) 3_655 . . 6_675 ?
Cs1 W1 O3 Cs1 -156.1(3) 8_474 . . 6_675 ?
Cs1 W1 O3 Cs1 175.0(8) 6_674 . . 6_675 ?
F3 W1 O3 Cs1 113.4(5) . . . . ?
O3 W1 O3 Cs1 -146.0(2) 3_655 . . . ?
F2 W1 O3 Cs1 -35.7(14) 3_655 . . . ?
F2 W1 O3 Cs1 16.9(4) . . . . ?
O2 W1 O3 Cs1 -60.9(4) . . . . ?
Cs1 W1 O3 Cs1 157.7(2) 5_445 . . . ?
Cs1 W1 O3 Cs1 111.9(4) 7_645 . . . ?
Cs1 W1 O3 Cs1 -107.4(3) 3_655 . . . ?
Cs1 W1 O3 Cs1 79.6(9) 8_474 . . . ?
Cs1 W1 O3 Cs1 50.6(3) 6_674 . . . ?
F3 W1 O3 Cs1 1.5(5) . . . 7_645 ?
O3 W1 O3 Cs1 102.1(4) 3_655 . . 7_645 ?
F2 W1 O3 Cs1 -147.6(11) 3_655 . . 7_645 ?
F2 W1 O3 Cs1 -95.0(3) . . . 7_645 ?
O2 W1 O3 Cs1 -172.8(4) . . . 7_645 ?
Cs1 W1 O3 Cs1 45.8(3) 5_445 . . 7_645 ?
Cs1 W1 O3 Cs1 -111.9(4) . . . 7_645 ?
Cs1 W1 O3 Cs1 140.7(2) 3_655 . . 7_645 ?
Cs1 W1 O3 Cs1 -32.3(9) 8_474 . . 7_645 ?
Cs1 W1 O3 Cs1 -61.3(2) 6_674 . . 7_645 ?
O3 W1 F3 Cs1 1.8(6) 3_655 . . 5_445 ?
O3 W1 F3 Cs1 102.0(5) . . . 5_445 ?
F2 W1 F3 Cs1 -87.3(5) 3_655 . . 5_445 ?
F2 W1 F3 Cs1 -168.9(4) . . . 5_445 ?
Cs1 W1 F3 Cs1 103.8(8) 7_645 . . 5_445 ?
Cs1 W1 F3 Cs1 152.3(2) . . . 5_445 ?
Cs1 W1 F3 Cs1 -48.5(6) 3_655 . . 5_445 ?
Cs1 W1 F3 Cs1 -92.5(3) 8_474 . . 5_445 ?
Cs1 W1 F3 Cs1 -163.7(6) 6_674 . . 5_445 ?
O3 W1 F3 Cs1 -102.0(5) 3_655 . . 7_645 ?
O3 W1 F3 Cs1 -1.8(6) . . . 7_645 ?
F2 W1 F3 Cs1 168.9(4) 3_655 . . 7_645 ?
F2 W1 F3 Cs1 87.3(5) . . . 7_645 ?
Cs1 W1 F3 Cs1 -103.8(8) 5_445 . . 7_645 ?
Cs1 W1 F3 Cs1 48.5(6) . . . 7_645 ?
Cs1 W1 F3 Cs1 -152.3(2) 3_655 . . 7_645 ?
Cs1 W1 F3 Cs1 163.7(6) 8_474 . . 7_645 ?
Cs1 W1 F3 Cs1 92.5(3) 6_674 . . 7_645 ?

_refine_diff_density_max         1.367
_refine_diff_density_min         -1.188
_refine_diff_density_rms         0.265



####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_1
_database_code_depnum_ccdc_archive 'CCDC 2164004'
loop_
_audit_author_name
_audit_author_address
'Yilei Hu'
;Tongji University
China
;
_audit_update_record             
;
2022-04-11 deposited with the CCDC.	2022-07-26 downloaded from the CCDC.
;

_audit_creation_method           SHELXL-2017/1
_shelx_SHELXL_version_number     2017/1
_chemical_name_systematic        ?
_chemical_name_common            ?
_chemical_melting_point          ?
_chemical_formula_moiety         ?
_chemical_formula_sum            'F5 I O4 Rb2 W'
_chemical_formula_weight         640.69

loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
I I -0.4742 1.8119 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Rb Rb -0.9393 2.9676 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
W W -0.8490 6.8722 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_space_group_crystal_system      orthorhombic
_space_group_IT_number           36
_space_group_name_H-M_alt        'C m c 21'
_space_group_name_Hall           'C 2c -2'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;

loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, z+1/2'
'-x, y, z'
'x, -y, z+1/2'
'x+1/2, y+1/2, z'
'-x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z'
'x+1/2, -y+1/2, z+1/2'

_cell_length_a                   11.726(2)
_cell_length_b                   10.188(2)
_cell_length_c                   7.6661(16)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     915.8(3)
_cell_formula_units_Z            4
_cell_measurement_temperature    296(2)
_cell_measurement_reflns_used    3604
_cell_measurement_theta_min      2.648
_cell_measurement_theta_max      24.978

_exptl_crystal_description       plate
_exptl_crystal_colour            colorless
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_density_diffrn    4.647
_exptl_crystal_F_000             1112
_exptl_transmission_factor_min   0.4566
_exptl_transmission_factor_max   0.8014
_exptl_crystal_size_max          0.3
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.1
_exptl_absorpt_coefficient_mu    26.607
_shelx_estimated_absorpt_T_min   ?
_shelx_estimated_absorpt_T_max   ?
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_special_details   ?
_diffrn_ambient_temperature      296(2)
_diffrn_radiation_wavelength     0.71073
_diffrn_radiation_type           MoK\a
_diffrn_source                   ?
_diffrn_measurement_device_type  'CCD area detector'
_diffrn_measurement_method       multi-scan
_diffrn_detector_area_resol_mean ?
_diffrn_reflns_number            3604
_diffrn_reflns_av_unetI/netI     0.0501
_diffrn_reflns_av_R_equivalents  0.0563
_diffrn_reflns_limit_h_min       -13
_diffrn_reflns_limit_h_max       13
_diffrn_reflns_limit_k_min       -12
_diffrn_reflns_limit_k_max       12
_diffrn_reflns_limit_l_min       -9
_diffrn_reflns_limit_l_max       9
_diffrn_reflns_theta_min         2.648
_diffrn_reflns_theta_max         24.978
_diffrn_reflns_theta_full        24.978
_diffrn_measured_fraction_theta_max 0.985
_diffrn_measured_fraction_theta_full 0.985
_diffrn_reflns_Laue_measured_fraction_max 0.985
_diffrn_reflns_Laue_measured_fraction_full 0.985
_diffrn_reflns_point_group_measured_fraction_max 0.992
_diffrn_reflns_point_group_measured_fraction_full 0.992
_reflns_number_total             821
_reflns_number_gt                816
_reflns_threshold_expression     'I > 2σ(I)'
_reflns_Friedel_coverage         0.856
_reflns_Friedel_fraction_max     1.000
_reflns_Friedel_fraction_full    1.000

_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  'SHELXL-2017/1 (Sheldrick, 2017)'
_computing_molecular_graphics    ?
_computing_publication_material  ?
_refine_special_details          
;
 Refined as a 2-component inversion twin.
;
_refine_ls_structure_factor_coef Fsqd
_refine_ls_matrix_type           full
_refine_ls_weighting_scheme      calc
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0002P)²+550.2583P] where P=(Fo²+2Fc²)/3'
_atom_sites_solution_primary     ?
_atom_sites_solution_secondary   ?
_atom_sites_solution_hydrogens   .
_refine_ls_hydrogen_treatment    undef
_refine_ls_extinction_method     none
_refine_ls_extinction_coef       .
_refine_ls_abs_structure_details 
;
 Refined as an inversion twin.
;
_refine_ls_abs_structure_Flack   0.32(10)
_chemical_absolute_configuration ?
_refine_ls_number_reflns         821
_refine_ls_number_parameters     71
_refine_ls_number_restraints     37
_refine_ls_R_factor_all          0.0774
_refine_ls_R_factor_gt           0.0773
_refine_ls_wR_factor_ref         0.1834
_refine_ls_wR_factor_gt          0.1834
_refine_ls_goodness_of_fit_ref   1.020
_refine_ls_restrained_S_all      0.995
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000

loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
W1 W 0.000000 0.1616(3) 0.4355(2) 0.0256(9) Uani 1 2 d S T P . .
I1A I 0.000000 0.4766(5) 0.1638(7) 0.0142(11) Uani 0.9 2 d S T P . .
I1B I -0.044(5) 0.530(7) 0.201(8) 0.0142(11) Uani 0.05 1 d . . P . .
F1 F 0.165(4) 0.468(5) 0.163(9) 0.076(13) Uani 1 1 d . U . . .
F2 F 0.108(3) 0.236(4) 0.605(5) 0.045(9) Uani 1 1 d . U . . .
O3 O 0.118(4) 0.159(4) 0.286(6) 0.043(11) Uani 1 1 d . U . . .
O1 O 0.000000 0.355(9) 0.006(10) 0.07(2) Uani 1 2 d S TU P . .
O2 O 0.000000 0.376(5) 0.364(7) 0.021(11) Uani 1 2 d S TU P . .
F3 F 0.000000 0.006(8) 0.506(10) 0.078(19) Uani 1 2 d S TU P . .
Rb1 Rb 0.3061(4) 0.3368(7) 0.4323(11) 0.0417(15) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W1 F3 1.67(8) . ?
W1 O3 1.80(5) 3 ?
W1 O3 1.80(5) . ?
W1 F2 1.97(4) . ?
W1 F2 1.97(4) 3 ?
W1 O2 2.25(5) . ?
W1 Rb1 4.009(5) . ?
W1 Rb1 4.009(5) 3 ?
W1 Rb1 4.015(6) 5_445 ?
W1 Rb1 4.015(6) 7_545 ?
I1A I1B 0.80(7) 3 ?
I1A I1B 0.80(7) . ?
I1A O1 1.73(9) . ?
I1A O2 1.84(5) . ?
I1A F1 1.93(4) . ?
I1A F1 1.93(4) 3 ?
I1A Rb1 4.303(9) 8_454 ?
I1A Rb1 4.303(9) 6_554 ?
I1B I1B 1.04(12) 3 ?
I1B F1 1.57(7) 3 ?
I1B O2 2.07(8) . ?
I1B O1 2.38(11) . ?
I1B Rb1 3.94(6) 2_564 ?
I1B Rb1 4.00(7) 5_455 ?
I1B Rb1 4.05(6) 3 ?
F1 Rb1 2.96(6) . ?
F1 Rb1 3.14(6) 4_564 ?
F1 Rb1 3.59(5) 6_554 ?
F2 Rb1 2.80(4) 6 ?
F2 Rb1 2.87(4) . ?
O3 Rb1 2.85(5) 6_554 ?
O3 Rb1 3.07(5) . ?
O3 Rb1 3.58(5) 7_545 ?
O1 Rb1 3.05(6) 8_454 ?
O1 Rb1 3.05(6) 6_554 ?
F3 Rb1 2.91(5) 5_445 ?
F3 Rb1 2.91(5) 7_545 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
F3 W1 O3 101(2) . 3 ?
F3 W1 O3 101(2) . . ?
O3 W1 O3 101(3) 3 . ?
F3 W1 F2 99(2) . . ?
O3 W1 F2 157.6(18) 3 . ?
O3 W1 F2 86.1(17) . . ?
F3 W1 F2 99(2) . 3 ?
O3 W1 F2 86.1(17) 3 3 ?
O3 W1 F2 157.6(18) . 3 ?
F2 W1 F2 80(2) . 3 ?
F3 W1 O2 175(3) . . ?
O3 W1 O2 81.9(16) 3 . ?
O3 W1 O2 81.9(16) . . ?
F2 W1 O2 77.9(15) . . ?
F2 W1 O2 77.9(15) 3 . ?
F3 W1 Rb1 115.0(4) . . ?
O3 W1 Rb1 133.8(15) 3 . ?
O3 W1 Rb1 46.6(14) . . ?
F2 W1 Rb1 42.0(12) . . ?
F2 W1 Rb1 114.2(12) 3 . ?
O2 W1 Rb1 64.32(18) . . ?
F3 W1 Rb1 115.0(4) . 3 ?
O3 W1 Rb1 46.6(14) 3 3 ?
O3 W1 Rb1 133.8(15) . 3 ?
F2 W1 Rb1 114.2(12) . 3 ?
F2 W1 Rb1 42.0(12) 3 3 ?
O2 W1 Rb1 64.32(18) . 3 ?
Rb1 W1 Rb1 127.1(2) . 3 ?
F3 W1 Rb1 38.9(12) . 5_445 ?
O3 W1 Rb1 63.1(14) 3 5_445 ?
O3 W1 Rb1 114.8(14) . 5_445 ?
F2 W1 Rb1 133.2(11) . 5_445 ?
F2 W1 Rb1 87.4(11) 3 5_445 ?
O2 W1 Rb1 142.9(5) . 5_445 ?
Rb1 W1 Rb1 150.92(19) . 5_445 ?
Rb1 W1 Rb1 81.95(4) 3 5_445 ?
F3 W1 Rb1 38.9(12) . 7_545 ?
O3 W1 Rb1 114.8(14) 3 7_545 ?
O3 W1 Rb1 63.1(14) . 7_545 ?
F2 W1 Rb1 87.4(11) . 7_545 ?
F2 W1 Rb1 133.2(11) 3 7_545 ?
O2 W1 Rb1 142.9(5) . 7_545 ?
Rb1 W1 Rb1 81.95(4) . 7_545 ?
Rb1 W1 Rb1 150.92(19) 3 7_545 ?
Rb1 W1 Rb1 68.97(18) 5_445 7_545 ?
I1B I1A I1B 81(8) 3 . ?
I1B I1A O1 137(4) 3 . ?
I1B I1A O1 137(4) . . ?
I1B I1A O2 94(5) 3 . ?
I1B I1A O2 94(5) . . ?
O1 I1A O2 101(3) . . ?
I1B I1A F1 52(4) 3 . ?
I1B I1A F1 133(4) . . ?
O1 I1A F1 88.0(17) . . ?
O2 I1A F1 89(2) . . ?
I1B I1A F1 133(4) 3 3 ?
I1B I1A F1 52(4) . 3 ?
O1 I1A F1 88.0(17) . 3 ?
O2 I1A F1 89(2) . 3 ?
F1 I1A F1 175(3) . 3 ?
I1B I1A Rb1 172(4) 3 8_454 ?
I1B I1A Rb1 108(4) . 8_454 ?
O1 I1A Rb1 35.0(11) . 8_454 ?
O2 I1A Rb1 86.0(14) . 8_454 ?
F1 I1A Rb1 119.5(16) . 8_454 ?
F1 I1A Rb1 55.7(15) 3 8_454 ?
I1B I1A Rb1 108(4) 3 6_554 ?
I1B I1A Rb1 172(4) . 6_554 ?
O1 I1A Rb1 35.0(11) . 6_554 ?
O2 I1A Rb1 86.0(14) . 6_554 ?
F1 I1A Rb1 55.7(15) . 6_554 ?
F1 I1A Rb1 119.5(16) 3 6_554 ?
Rb1 I1A Rb1 63.79(16) 8_454 6_554 ?
I1A I1B I1B 50(4) . 3 ?
I1A I1B F1 104(6) . 3 ?
I1B I1B F1 154(3) 3 3 ?
I1A I1B O2 63(4) . . ?
I1B I1B O2 75.5(17) 3 . ?
F1 I1B O2 92(4) 3 . ?
I1A I1B O1 30(3) . . ?
I1B I1B O1 77.4(15) 3 . ?
F1 I1B O1 77(3) 3 . ?
O2 I1B O1 76(3) . . ?
I1A I1B Rb1 123(5) . 2_564 ?
I1B I1B Rb1 141.2(9) 3 2_564 ?
F1 I1B Rb1 49(3) 3 2_564 ?
O2 I1B Rb1 141(2) . 2_564 ?
O1 I1B Rb1 96(2) . 2_564 ?
I1A I1B Rb1 166(5) . 5_455 ?
I1B I1B Rb1 116.0(8) 3 5_455 ?
F1 I1B Rb1 90(3) 3 5_455 ?
O2 I1B Rb1 116(3) . 5_455 ?
O1 I1B Rb1 163(3) . 5_455 ?
Rb1 I1B Rb1 67.6(11) 2_564 5_455 ?
I1A I1B Rb1 109(5) . 3 ?
I1B I1B Rb1 139.3(9) 3 3 ?
F1 I1B Rb1 37(3) 3 3 ?
O2 I1B Rb1 63.9(16) . 3 ?
O1 I1B Rb1 94(2) . 3 ?
Rb1 I1B Rb1 78.8(11) 2_564 3 ?
Rb1 I1B Rb1 81.6(13) 5_455 3 ?
I1B F1 I1A 24(3) 3 . ?
I1B F1 Rb1 124(4) 3 . ?
I1A F1 Rb1 125(3) . . ?
I1B F1 Rb1 109(4) 3 4_564 ?
I1A F1 Rb1 120(3) . 4_564 ?
Rb1 F1 Rb1 112.5(14) . 4_564 ?
I1B F1 Rb1 122(4) 3 6_554 ?
I1A F1 Rb1 97.9(18) . 6_554 ?
Rb1 F1 Rb1 84.3(12) . 6_554 ?
Rb1 F1 Rb1 102.7(17) 4_564 6_554 ?
W1 F2 Rb1 136.3(18) . 6 ?
W1 F2 Rb1 110.7(17) . . ?
Rb1 F2 Rb1 102.6(13) 6 . ?
W1 O3 Rb1 148(2) . 6_554 ?
W1 O3 Rb1 108.1(19) . . ?
Rb1 O3 Rb1 96.6(14) 6_554 . ?
W1 O3 Rb1 90.3(17) . 7_545 ?
Rb1 O3 Rb1 103.6(13) 6_554 7_545 ?
Rb1 O3 Rb1 104.4(13) . 7_545 ?
I1A O1 I1B 13.3(16) . . ?
I1A O1 I1B 13.3(16) . 3 ?
I1B O1 I1B 25(3) . 3 ?
I1A O1 Rb1 126.1(19) . 8_454 ?
I1B O1 Rb1 115.7(18) . 8_454 ?
I1B O1 Rb1 139(3) 3 8_454 ?
I1A O1 Rb1 126.1(19) . 6_554 ?
I1B O1 Rb1 139(3) . 6_554 ?
I1B O1 Rb1 115.7(18) 3 6_554 ?
Rb1 O1 Rb1 96(3) 8_454 6_554 ?
I1A O2 I1B 22.7(19) . . ?
I1A O2 I1B 22.7(19) . 3 ?
I1B O2 I1B 29(3) . 3 ?
I1A O2 W1 138(3) . . ?
I1B O2 W1 152(3) . . ?
I1B O2 W1 152(3) 3 . ?
W1 F3 Rb1 120(2) . 5_445 ?
W1 F3 Rb1 120(2) . 7_545 ?
Rb1 F3 Rb1 103(3) 5_445 7_545 ?
F2 Rb1 O3 138.0(12) 6_554 6 ?
F2 Rb1 F2 127.6(9) 6_554 . ?
O3 Rb1 F2 79.5(12) 6 . ?
F2 Rb1 F3 92.9(16) 6_554 5 ?
O3 Rb1 F3 64.1(18) 6 5 ?
F2 Rb1 F3 139.1(17) . 5 ?
F2 Rb1 F1 72.3(14) 6_554 . ?
O3 Rb1 F1 145.9(14) 6 . ?
F2 Rb1 F1 91.7(14) . . ?
F3 Rb1 F1 107.8(18) 5 . ?
F2 Rb1 O1 74.4(17) 6_554 6 ?
O3 Rb1 O1 66.5(18) 6 6 ?
F2 Rb1 O1 106.6(15) . 6 ?
F3 Rb1 O1 76.3(19) 5 6 ?
F1 Rb1 O1 146.6(19) . 6 ?
F2 Rb1 O3 77.0(12) 6_554 . ?
O3 Rb1 O3 125.5(12) 6 . ?
F2 Rb1 O3 51.3(11) . . ?
F3 Rb1 O3 169.5(18) 5 . ?
F1 Rb1 O3 67.0(13) . . ?
O1 Rb1 O3 102.9(17) 6 . ?
F2 Rb1 F1 149.5(14) 6_554 4_565 ?
O3 Rb1 F1 67.6(15) 6 4_565 ?
F2 Rb1 F1 62.6(11) . 4_565 ?
F3 Rb1 F1 85.8(16) 5 4_565 ?
F1 Rb1 F1 79.1(8) . 4_565 ?
O1 Rb1 F1 134.0(19) 6 4_565 ?
O3 Rb1 F1 101.7(13) . 4_565 ?
F2 Rb1 O3 82.6(11) 6_554 7 ?
O3 Rb1 O3 101.9(11) 6 7 ?
F2 Rb1 O3 132.5(11) . 7 ?
F3 Rb1 O3 47.4(16) 5 7 ?
F1 Rb1 O3 60.5(12) . 7 ?
O1 Rb1 O3 117.5(16) 6 7 ?
O3 Rb1 O3 127.2(14) . 7 ?
F1 Rb1 O3 74.1(12) 4_565 7 ?
F2 Rb1 F1 100.4(14) 6_554 6 ?
O3 Rb1 F1 60.9(14) 6 6 ?
F2 Rb1 F1 62.5(11) . 6 ?
F3 Rb1 F1 110.0(17) 5 6 ?
F1 Rb1 F1 141.8(8) . 6 ?
O1 Rb1 F1 44.2(15) 6 6 ?
O3 Rb1 F1 74.8(12) . 6 ?
F1 Rb1 F1 108.7(18) 4_565 6 ?
O3 Rb1 F1 157.4(11) 7 6 ?
F2 Rb1 I1B 147.1(13) 6_554 2_565 ?
O3 Rb1 I1B 74.9(13) 6 2_565 ?
F2 Rb1 I1B 41.5(12) . 2_565 ?
F3 Rb1 I1B 107.6(16) 5 2_565 ?
F1 Rb1 I1B 76.8(15) . 2_565 ?
O1 Rb1 I1B 134.8(18) 6 2_565 ?
O3 Rb1 I1B 80.6(13) . 2_565 ?
F1 Rb1 I1B 22.2(13) 4_565 2_565 ?
O3 Rb1 I1B 92.3(12) 7 2_565 ?
F1 Rb1 I1B 96.6(13) 6 2_565 ?
F2 Rb1 I1B 40.6(12) 6_554 5_545 ?
O3 Rb1 I1B 107.2(13) 6 5_545 ?
F2 Rb1 I1B 106.2(12) . 5_545 ?
F3 Rb1 I1B 102.0(15) 5 5_545 ?
F1 Rb1 I1B 106.8(14) . 5_545 ?
O1 Rb1 I1B 41.8(17) 6 5_545 ?
O3 Rb1 I1B 72.0(12) . 5_545 ?
F1 Rb1 I1B 167.9(13) 4_565 5_545 ?
O3 Rb1 I1B 118.0(12) 7 5_545 ?
F1 Rb1 I1B 60.0(14) 6 5_545 ?
I1B Rb1 I1B 147.5(6) 2_565 5_545 ?

loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion_publ_flag
O1 I1A I1B I1B -156(9) . . . 3 ?
O2 I1A I1B I1B 94(4) . . . 3 ?
F1 I1A I1B I1B 2(3) . . . 3 ?
F1 I1A I1B I1B 178(3) 3 . . 3 ?
Rb1 I1A I1B I1B -179(5) 8_454 . . 3 ?
I1B I1A I1B F1 -178(3) 3 . . 3 ?
O1 I1A I1B F1 26(9) . . . 3 ?
O2 I1A I1B F1 -85(5) . . . 3 ?
F1 I1A I1B F1 -177(6) . . . 3 ?
Rb1 I1A I1B F1 2(6) 8_454 . . 3 ?
I1B I1A I1B O2 -94(4) 3 . . . ?
O1 I1A I1B O2 111(6) . . . . ?
F1 I1A I1B O2 -92(5) . . . . ?
F1 I1A I1B O2 85(5) 3 . . . ?
Rb1 I1A I1B O2 87.2(18) 8_454 . . . ?
I1B I1A I1B O1 156(9) 3 . . . ?
O2 I1A I1B O1 -111(6) . . . . ?
F1 I1A I1B O1 157(10) . . . . ?
F1 I1A I1B O1 -26(9) 3 . . . ?
Rb1 I1A I1B O1 -23(5) 8_454 . . . ?
I1B I1A I1B Rb1 132(3) 3 . . 2_564 ?
O1 I1A I1B Rb1 -24(10) . . . 2_564 ?
O2 I1A I1B Rb1 -135(4) . . . 2_564 ?
F1 I1A I1B Rb1 133(4) . . . 2_564 ?
F1 I1A I1B Rb1 -50(4) 3 . . 2_564 ?
Rb1 I1A I1B Rb1 -47(5) 8_454 . . 2_564 ?
I1B I1A I1B Rb1 -5(25) 3 . . 5_455 ?
O1 I1A I1B Rb1 -161(17) . . . 5_455 ?
O2 I1A I1B Rb1 88(21) . . . 5_455 ?
F1 I1A I1B Rb1 -4(25) . . . 5_455 ?
F1 I1A I1B Rb1 173(25) 3 . . 5_455 ?
Rb1 I1A I1B Rb1 176(20) 8_454 . . 5_455 ?
I1B I1A I1B Rb1 -140(2) 3 . . 3 ?
O1 I1A I1B Rb1 65(7) . . . 3 ?
O2 I1A I1B Rb1 -46(3) . . . 3 ?
F1 I1A I1B Rb1 -138(4) . . . 3 ?
F1 I1A I1B Rb1 39(3) 3 . . 3 ?
Rb1 I1A I1B Rb1 41(3) 8_454 . . 3 ?
F3 W1 O3 Rb1 108(4) . . . 6_554 ?
O3 W1 O3 Rb1 4(6) 3 . . 6_554 ?
F2 W1 O3 Rb1 -154(4) . . . 6_554 ?
F2 W1 O3 Rb1 -102(6) 3 . . 6_554 ?
O2 W1 O3 Rb1 -76(4) . . . 6_554 ?
Rb1 W1 O3 Rb1 -138(5) . . . 6_554 ?
Rb1 W1 O3 Rb1 -34(5) 3 . . 6_554 ?
Rb1 W1 O3 Rb1 69(4) 5_445 . . 6_554 ?
Rb1 W1 O3 Rb1 117(4) 7_545 . . 6_554 ?
F3 W1 O3 Rb1 -114(2) . . . . ?
O3 W1 O3 Rb1 142.2(11) 3 . . . ?
F2 W1 O3 Rb1 -16.2(17) . . . . ?
F2 W1 O3 Rb1 36(6) 3 . . . ?
O2 W1 O3 Rb1 62.1(16) . . . . ?
Rb1 W1 O3 Rb1 104.1(18) 3 . . . ?
Rb1 W1 O3 Rb1 -152.6(9) 5_445 . . . ?
Rb1 W1 O3 Rb1 -105.3(18) 7_545 . . . ?
F3 W1 O3 Rb1 -9(2) . . . 7_545 ?
O3 W1 O3 Rb1 -112.5(16) 3 . . 7_545 ?
F2 W1 O3 Rb1 89.1(13) . . . 7_545 ?
F2 W1 O3 Rb1 141(5) 3 . . 7_545 ?
O2 W1 O3 Rb1 167.4(14) . . . 7_545 ?
Rb1 W1 O3 Rb1 105.3(18) . . . 7_545 ?
Rb1 W1 O3 Rb1 -150.6(9) 3 . . 7_545 ?
Rb1 W1 O3 Rb1 -47.3(13) 5_445 . . 7_545 ?
I1B I1A O1 I1B -143(14) 3 . . . ?
O2 I1A O1 I1B 108(7) . . . . ?
F1 I1A O1 I1B -164(7) . . . . ?
F1 I1A O1 I1B 20(8) 3 . . . ?
Rb1 I1A O1 I1B 41(9) 8_454 . . . ?
Rb1 I1A O1 I1B 175(7) 6_554 . . . ?
I1B I1A O1 I1B 143(14) . . . 3 ?
O2 I1A O1 I1B -108(7) . . . 3 ?
F1 I1A O1 I1B -20(8) . . . 3 ?
F1 I1A O1 I1B 164(7) 3 . . 3 ?
Rb1 I1A O1 I1B -175(7) 8_454 . . 3 ?
Rb1 I1A O1 I1B -41(9) 6_554 . . 3 ?
I1B I1A O1 Rb1 175(7) 3 . . 8_454 ?
I1B I1A O1 Rb1 -41(9) . . . 8_454 ?
O2 I1A O1 Rb1 67(4) . . . 8_454 ?
F1 I1A O1 Rb1 155(4) . . . 8_454 ?
F1 I1A O1 Rb1 -21(4) 3 . . 8_454 ?
Rb1 I1A O1 Rb1 134(8) 6_554 . . 8_454 ?
I1B I1A O1 Rb1 41(9) 3 . . 6_554 ?
I1B I1A O1 Rb1 -175(7) . . . 6_554 ?
O2 I1A O1 Rb1 -67(4) . . . 6_554 ?
F1 I1A O1 Rb1 21(4) . . . 6_554 ?
F1 I1A O1 Rb1 -155(4) 3 . . 6_554 ?
Rb1 I1A O1 Rb1 -134(8) 8_454 . . 6_554 ?
I1B I1A O2 I1B 81(8) 3 . . . ?
O1 I1A O2 I1B -140(4) . . . . ?
F1 I1A O2 I1B 133(4) . . . . ?
F1 I1A O2 I1B -52(4) 3 . . . ?
Rb1 I1A O2 I1B -108(4) 8_454 . . . ?
Rb1 I1A O2 I1B -172(4) 6_554 . . . ?
I1B I1A O2 I1B -81(8) . . . 3 ?
O1 I1A O2 I1B 140(4) . . . 3 ?
F1 I1A O2 I1B 52(4) . . . 3 ?
F1 I1A O2 I1B -133(4) 3 . . 3 ?
Rb1 I1A O2 I1B 172(4) 8_454 . . 3 ?
Rb1 I1A O2 I1B 108(4) 6_554 . . 3 ?
I1B I1A O2 W1 -140(4) 3 . . . ?
I1B I1A O2 W1 140(4) . . . . ?
O1 I1A O2 W1 0.000(8) . . . . ?
F1 I1A O2 W1 -87.7(16) . . . . ?
F1 I1A O2 W1 87.7(16) 3 . . . ?
Rb1 I1A O2 W1 31.98(11) 8_454 . . . ?
Rb1 I1A O2 W1 -31.98(11) 6_554 . . . ?
O3 W1 F3 Rb1 -13(4) 3 . . 5_445 ?
O3 W1 F3 Rb1 -116(3) . . . 5_445 ?
F2 W1 F3 Rb1 156(3) . . . 5_445 ?
F2 W1 F3 Rb1 75(3) 3 . . 5_445 ?
Rb1 W1 F3 Rb1 -163.1(18) . . . 5_445 ?
Rb1 W1 F3 Rb1 34(4) 3 . . 5_445 ?
Rb1 W1 F3 Rb1 -129(6) 7_545 . . 5_445 ?
O3 W1 F3 Rb1 116(3) 3 . . 7_545 ?
O3 W1 F3 Rb1 13(4) . . . 7_545 ?
F2 W1 F3 Rb1 -75(3) . . . 7_545 ?
F2 W1 F3 Rb1 -156(3) 3 . . 7_545 ?
Rb1 W1 F3 Rb1 -34(4) . . . 7_545 ?
Rb1 W1 F3 Rb1 163.1(18) 3 . . 7_545 ?
Rb1 W1 F3 Rb1 129(6) 5_445 . . 7_545 ?

_refine_diff_density_max         4.248
_refine_diff_density_min         -5.754
_refine_diff_density_rms         0.630



# start Validation Reply Form
_vrf_PLAT241_1                   
;
PROBLEM:  'MainMol' Ueq as Compared to Neighbors of ........ O1 Check
RESPONSE: This may be due to the disorder of [IO2F2] unit. 


;
# end Validation Reply Form
